LMucko/crystallography-open-database huggingface dataset:
Increase in Al-Si and Na-Ca disorder with temperature in scapolite Me32.9 Note: T = 405 C Note: 32.9% Meionite, 67.1% Marialite
Antao, S. M.; Hassan, I.; The Canadian Mineralogist 46 (2008) 1577–1591; doi:10.3749/canmin.46.5.1577

data_9013346
_publ_section_title
;
 Increase in Al-Si and Na-Ca disorder with temperature in scapolite Me32.9
 Note: T = 405 C
 Note: 32.9% Meionite, 67.1% Marialite
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1577
_journal_page_last               1591
_journal_paper_doi               10.3749/canmin.46.5.1577
_journal_volume                  46
_journal_year                    2008
_chemical_compound_source        'Monmouth Township, Ontario, Canada'
_chemical_formula_sum
'C0.24 Al3.56 Ca1.24 Cl0.76 Na2.76 O28 Si8.44'
_chemical_name_mineral           Marialite
_space_group_IT_number           86
_symmetry_space_group_name_Hall  '-P 4bc'
_symmetry_space_group_name_H-M   'P 42/n :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   12.1172
_cell_length_b                   12.1172
_cell_length_c                   7.5800
_cell_formula_units_Z            2
_cell_volume                     1112.945
_database_code_amcsd             0006237
_diffrn_ambient_temperature      678.15
_exptl_crystal_density_diffrn    2.757
_cod_original_sg_symbol_H-M      'P 42/n'
_cod_original_formula_sum
'(Ca1.24 Na2.76) Si8.44 Al3.56 O28 (C.24 Cl.76)'
_cod_database_code               9013346
Increase in Al-Si and Na-Ca disorder with temperature in scapolite Me32.9 Note: T = 505 C Note: 32.9% Meionite, 67.1% Marialite
Antao, S. M.; Hassan, I.; The Canadian Mineralogist 46 (2008) 1577–1591; doi:10.3749/canmin.46.5.1577

data_9013347
_publ_section_title
;
 Increase in Al-Si and Na-Ca disorder with temperature in scapolite Me32.9
 Note: T = 505 C
 Note: 32.9% Meionite, 67.1% Marialite
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1577
_journal_page_last               1591
_journal_paper_doi               10.3749/canmin.46.5.1577
_journal_volume                  46
_journal_year                    2008
_chemical_compound_source        'Monmouth Township, Ontario, Canada'
_chemical_formula_sum
'C0.24 Al3.56 Ca1.24 Cl0.76 Na2.76 O28 Si8.44'
_chemical_name_mineral           Marialite
_space_group_IT_number           86
_symmetry_space_group_name_Hall  '-P 4bc'
_symmetry_space_group_name_H-M   'P 42/n :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   12.1335
_cell_length_b                   12.1335
_cell_length_c                   7.5801
_cell_formula_units_Z            2
_cell_volume                     1115.956
_database_code_amcsd             0006238
_diffrn_ambient_temperature      778.15
_exptl_crystal_density_diffrn    2.750
_cod_original_sg_symbol_H-M      'P 42/n'
_cod_original_formula_sum
'(Ca1.24 Na2.76) Si8.44 Al3.56 O28 (C.24 Cl.76)'
_cod_database_code               9013347
Increase in Al-Si and Na-Ca disorder with temperature in scapolite Me32.9 Note: T = 603 C Note: 32.9% Meionite, 67.1% Marialite
Antao, S. M.; Hassan, I.; The Canadian Mineralogist 46 (2008) 1577–1591; doi:10.3749/canmin.46.5.1577

data_9013348
_publ_section_title
;
 Increase in Al-Si and Na-Ca disorder with temperature in scapolite Me32.9
 Note: T = 603 C
 Note: 32.9% Meionite, 67.1% Marialite
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1577
_journal_page_last               1591
_journal_paper_doi               10.3749/canmin.46.5.1577
_journal_volume                  46
_journal_year                    2008
_chemical_compound_source        'Monmouth Township, Ontario, Canada'
_chemical_formula_sum
'C0.24 Al3.56 Ca1.24 Cl0.76 Na2.76 O28 Si8.44'
_chemical_name_mineral           Marialite
_space_group_IT_number           86
_symmetry_space_group_name_Hall  '-P 4bc'
_symmetry_space_group_name_H-M   'P 42/n :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   12.1510
_cell_length_b                   12.1510
_cell_length_c                   7.5800
_cell_formula_units_Z            2
_cell_volume                     1119.163
_database_code_amcsd             0006239
_diffrn_ambient_temperature      876.15
_exptl_crystal_density_diffrn    2.742
_cod_original_sg_symbol_H-M      'P 42/n'
_cod_original_formula_sum
'(Ca1.24 Na2.76) Si8.44 Al3.56 O28 (C.24 Cl.76)'
_cod_database_code               9013348
Increase in Al-Si and Na-Ca disorder with temperature in scapolite Me32.9 Note: T = 702 C Note: 32.9% Meionite, 67.1% Marialite
Antao, S. M.; Hassan, I.; The Canadian Mineralogist 46 (2008) 1577–1591; doi:10.3749/canmin.46.5.1577

data_9013349
_publ_section_title
;
 Increase in Al-Si and Na-Ca disorder with temperature in scapolite Me32.9
 Note: T = 702 C
 Note: 32.9% Meionite, 67.1% Marialite
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1577
_journal_page_last               1591
_journal_paper_doi               10.3749/canmin.46.5.1577
_journal_volume                  46
_journal_year                    2008
_chemical_compound_source        'Monmouth Township, Ontario, Canada'
_chemical_formula_sum
'C0.24 Al3.56 Ca1.24 Cl0.76 Na2.76 O28 Si8.44'
_chemical_name_mineral           Marialite
_space_group_IT_number           86
_symmetry_space_group_name_Hall  '-P 4bc'
_symmetry_space_group_name_H-M   'P 42/n :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   12.1673
_cell_length_b                   12.1673
_cell_length_c                   7.5799
_cell_formula_units_Z            2
_cell_volume                     1122.153
_database_code_amcsd             0006240
_diffrn_ambient_temperature      975.15
_exptl_crystal_density_diffrn    2.735
_cod_original_sg_symbol_H-M      'P 42/n'
_cod_original_formula_sum
'(Ca1.24 Na2.76) Si8.44 Al3.56 O28 (C.24 Cl.76)'
_cod_database_code               9013349
Increase in Al-Si and Na-Ca disorder with temperature in scapolite Me32.9 Note: T = 801 C Note: 32.9% Meionite, 67.1% Marialite
Antao, S. M.; Hassan, I.; The Canadian Mineralogist 46 (2008) 1577–1591; doi:10.3749/canmin.46.5.1577

data_9013350
_publ_section_title
;
 Increase in Al-Si and Na-Ca disorder with temperature in scapolite Me32.9
 Note: T = 801 C
 Note: 32.9% Meionite, 67.1% Marialite
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1577
_journal_page_last               1591
_journal_paper_doi               10.3749/canmin.46.5.1577
_journal_volume                  46
_journal_year                    2008
_chemical_compound_source        'Monmouth Township, Ontario, Canada'
_chemical_formula_sum
'C0.24 Al3.56 Ca1.24 Cl0.76 Na2.76 O28 Si8.44'
_chemical_name_mineral           Marialite
_space_group_IT_number           86
_symmetry_space_group_name_Hall  '-P 4bc'
_symmetry_space_group_name_H-M   'P 42/n :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   12.1844
_cell_length_b                   12.1844
_cell_length_c                   7.5799
_cell_formula_units_Z            2
_cell_volume                     1125.309
_database_code_amcsd             0006241
_diffrn_ambient_temperature      1074.15
_exptl_crystal_density_diffrn    2.727
_cod_original_sg_symbol_H-M      'P 42/n'
_cod_original_formula_sum
'(Ca1.24 Na2.76) Si8.44 Al3.56 O28 (C.24 Cl.76)'
_cod_database_code               9013350
Increase in Al-Si and Na-Ca disorder with temperature in scapolite Me32.9 Note: T = 902 C Note: 32.9% Meionite, 67.1% Marialite
Antao, S. M.; Hassan, I.; The Canadian Mineralogist 46 (2008) 1577–1591; doi:10.3749/canmin.46.5.1577

data_9013351
_publ_section_title
;
 Increase in Al-Si and Na-Ca disorder with temperature in scapolite Me32.9
 Note: T = 902 C
 Note: 32.9% Meionite, 67.1% Marialite
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1577
_journal_page_last               1591
_journal_paper_doi               10.3749/canmin.46.5.1577
_journal_volume                  46
_journal_year                    2008
_chemical_compound_source        'Monmouth Township, Ontario, Canada'
_chemical_formula_sum
'C0.24 Al4.48 Ca1.24 Cl0.76 Na2.76 O28 Si7.52'
_chemical_name_mineral           Marialite
_space_group_IT_number           86
_symmetry_space_group_name_Hall  '-P 4bc'
_symmetry_space_group_name_H-M   'P 42/n :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   12.1974
_cell_length_b                   12.1974
_cell_length_c                   7.5795
_cell_formula_units_Z            2
_cell_volume                     1127.652
_database_code_amcsd             0006242
_diffrn_ambient_temperature      1175.15
_exptl_crystal_density_diffrn    2.718
_cod_original_sg_symbol_H-M      'P 42/n'
_cod_original_formula_sum
'(Ca1.24 Na2.76) Si7.52 Al4.48 O28 (C.24 Cl.76)'
_cod_database_code               9013351
Powder neutron-diffraction studies of clinopyroxenes. I. The crystal structure and thermoelastic properties of jadeite between 1.5 and 270 K Locality: Hweka and Mamon mining district, Burma Note: T = 2.4 K
Knight, K. S.; Price, G. D.; The Canadian Mineralogist 46 (2008) 1593–1622; doi:10.3749/canmin.46.6.1593

data_9013352
_publ_section_title
;Powder neutron-diffraction studies of clinopyroxenes. I. The crystal
 structure and thermoelastic properties of jadeite between 1.5 and 270 K
 Locality: Hweka and Mamon mining district, Burma Note: T = 2.4 K
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1593
_journal_page_last               1622
_journal_paper_doi               10.3749/canmin.46.6.1593
_journal_volume                  46
_journal_year                    2008
_chemical_formula_structural     NaAl(Si2O6)
_chemical_formula_sum            'Al Na O6 Si2'
_chemical_name_mineral           Jadeite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.5641
_cell_angle_gamma                90
_cell_length_a                   9.41591
_cell_length_b                   8.55521
_cell_length_c                   5.22073
_cell_formula_units_Z            4
_cell_volume                     400.950
_diffrn_ambient_temperature      2.4
_exptl_crystal_density_diffrn    3.349
_cod_original_formula_sum        'Na Al Si2 O6'
_cod_database_code               9013352
Powder neutron-diffraction studies of clinopyroxenes. I. The crystal structure and thermoelastic properties of jadeite between 1.5 and 270 K Locality: Hweka and Mamon mining district, Burma Note: T = 10.3 K Note: b parameter changed from paper
Knight, K. S.; Price, G. D.; The Canadian Mineralogist 46 (2008) 1593–1622; doi:10.3749/canmin.46.6.1593

data_9013353
_publ_section_title
;Powder neutron-diffraction studies of clinopyroxenes. I. The crystal
 structure and thermoelastic properties of jadeite between 1.5 and 270 K
 Locality: Hweka and Mamon mining district, Burma Note: T = 10.3 K Note: b
 parameter changed from paper
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1593
_journal_page_last               1622
_journal_paper_doi               10.3749/canmin.46.6.1593
_journal_volume                  46
_journal_year                    2008
_chemical_formula_structural     NaAl(Si2O6)
_chemical_formula_sum            'Al Na O6 Si2'
_chemical_name_mineral           Jadeite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.5641
_cell_angle_gamma                90
_cell_length_a                   9.41591
_cell_length_b                   8.55521
_cell_formula_units_Z            4
_cell_length_c                   5.22073
_cell_volume                     400.950
_diffrn_ambient_temperature      10.3
_exptl_crystal_density_diffrn    3.349
_cod_original_formula_sum        'Na Al Si2 O6'
_cod_database_code               9013353
Powder neutron-diffraction studies of clinopyroxenes. I. The crystal structure and thermoelastic properties of jadeite between 1.5 and 270 K Locality: Hweka and Mamon mining district, Burma Note: T = 19.7 K
Knight, K. S.; Price, G. D.; The Canadian Mineralogist 46 (2008) 1593–1622; doi:10.3749/canmin.46.6.1593

data_9013354
_publ_section_title
;Powder neutron-diffraction studies of clinopyroxenes. I. The crystal
 structure and thermoelastic properties of jadeite between 1.5 and 270 K
 Locality: Hweka and Mamon mining district, Burma Note: T = 19.7 K
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1593
_journal_page_last               1622
_journal_paper_doi               10.3749/canmin.46.6.1593
_journal_volume                  46
_journal_year                    2008
_chemical_formula_structural     NaAl(Si2O6)
_chemical_formula_sum            'Al Na O6 Si2'
_chemical_name_mineral           Jadeite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.5641
_cell_angle_gamma                90
_cell_length_a                   9.41591
_cell_length_b                   8.55521
_cell_length_c                   5.22073
_cell_formula_units_Z            4
_cell_volume                     400.950
_diffrn_ambient_temperature      19.7
_exptl_crystal_density_diffrn    3.349
_cod_original_formula_sum        'Na Al Si2 O6'
_cod_database_code               9013354
Powder neutron-diffraction studies of clinopyroxenes. I. The crystal structure and thermoelastic properties of jadeite between 1.5 and 270 K Locality: Hweka and Mamon mining district, Burma Note: T = 29.5 K
Knight, K. S.; Price, G. D.; The Canadian Mineralogist 46 (2008) 1593–1622; doi:10.3749/canmin.46.6.1593

data_9013355
_publ_section_title
;Powder neutron-diffraction studies of clinopyroxenes. I. The crystal
 structure and thermoelastic properties of jadeite between 1.5 and 270 K
 Locality: Hweka and Mamon mining district, Burma Note: T = 29.5 K
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1593
_journal_page_last               1622
_journal_paper_doi               10.3749/canmin.46.6.1593
_journal_volume                  46
_journal_year                    2008
_chemical_formula_structural     NaAl(Si2O6)
_chemical_formula_sum            'Al Na O6 Si2'
_chemical_name_mineral           Jadeite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.5642
_cell_angle_gamma                90
_cell_length_a                   9.41591
_cell_length_b                   8.55521
_cell_length_c                   5.22073
_cell_formula_units_Z            4
_cell_volume                     400.950
_diffrn_ambient_temperature      29.5
_exptl_crystal_density_diffrn    3.349
_cod_original_formula_sum        'Na Al Si2 O6'
_cod_database_code               9013355
Powder neutron-diffraction studies of clinopyroxenes. I. The crystal structure and thermoelastic properties of jadeite between 1.5 and 270 K Locality: Hweka and Mamon mining district, Burma Note: T = 39.0 K
Knight, K. S.; Price, G. D.; The Canadian Mineralogist 46 (2008) 1593–1622; doi:10.3749/canmin.46.6.1593

data_9013356
_publ_section_title
;Powder neutron-diffraction studies of clinopyroxenes. I. The crystal
 structure and thermoelastic properties of jadeite between 1.5 and 270 K
 Locality: Hweka and Mamon mining district, Burma Note: T = 39.0 K
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1593
_journal_page_last               1622
_journal_paper_doi               10.3749/canmin.46.6.1593
_journal_volume                  46
_journal_year                    2008
_chemical_formula_structural     NaAl(Si2O6)
_chemical_formula_sum            'Al Na O6 Si2'
_chemical_name_mineral           Jadeite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.5645
_cell_angle_gamma                90
_cell_length_a                   9.41591
_cell_length_b                   8.55521
_cell_length_c                   5.22073
_cell_formula_units_Z            4
_cell_volume                     400.949
_diffrn_ambient_temperature      39
_exptl_crystal_density_diffrn    3.349
_cod_original_formula_sum        'Na Al Si2 O6'
_cod_database_code               9013356
Powder neutron-diffraction studies of clinopyroxenes. I. The crystal structure and thermoelastic properties of jadeite between 1.5 and 270 K
Knight, K. S.; Price, G. D.; The Canadian Mineralogist 46 (2008) 1593–1622; doi:10.3749/canmin.46.6.1593

data_9013357
_publ_section_title
;Powder neutron-diffraction studies of clinopyroxenes. I. The crystal
 structure and thermoelastic properties of jadeite between 1.5 and 270 K
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1593
_journal_page_last               1622
_journal_paper_doi               10.3749/canmin.46.6.1593
_journal_volume                  46
_journal_year                    2008
_chemical_compound_source        'Hweka and Mamon mining district, Burma'
_chemical_formula_structural     NaAl(Si2O6)
_chemical_formula_sum            'Al Na O6 Si2'
_chemical_name_mineral           Jadeite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.5650
_cell_angle_gamma                90
_cell_length_a                   9.41592
_cell_length_b                   8.55523
_cell_length_c                   5.22073
_cell_formula_units_Z            4
_cell_volume                     400.949
_database_code_amcsd             0006248
_diffrn_ambient_temperature      47.5
_exptl_crystal_density_diffrn    3.349
_cod_original_formula_sum        'Na Al Si2 O6'
_cod_database_code               9013357
Powder neutron-diffraction studies of clinopyroxenes. I. The crystal structure and thermoelastic properties of jadeite between 1.5 and 270 K Locality: Hweka and Mamon mining district, Burma Note: T = 55.1 K
Knight, K. S.; Price, G. D.; The Canadian Mineralogist 46 (2008) 1593–1622; doi:10.3749/canmin.46.6.1593

data_9013358
_publ_section_title
;Powder neutron-diffraction studies of clinopyroxenes. I. The crystal
 structure and thermoelastic properties of jadeite between 1.5 and 270 K
 Locality: Hweka and Mamon mining district, Burma Note: T = 55.1 K
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1593
_journal_page_last               1622
_journal_paper_doi               10.3749/canmin.46.6.1593
_journal_volume                  46
_journal_year                    2008
_chemical_formula_structural     NaAl(Si2O6)
_chemical_formula_sum            'Al Na O6 Si2'
_chemical_name_mineral           Jadeite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.5655
_cell_angle_gamma                90
_cell_length_a                   9.41594
_cell_length_b                   8.55527
_cell_length_c                   5.22074
_cell_formula_units_Z            4
_cell_volume                     400.952
_diffrn_ambient_temperature      55.1
_exptl_crystal_density_diffrn    3.349
_cod_original_formula_sum        'Na Al Si2 O6'
_cod_database_code               9013358
Powder neutron-diffraction studies of clinopyroxenes. I. The crystal structure and thermoelastic properties of jadeite between 1.5 and 270 K Locality: Hweka and Mamon mining district, Burma Note: T = 64.0 K
Knight, K. S.; Price, G. D.; The Canadian Mineralogist 46 (2008) 1593–1622; doi:10.3749/canmin.46.6.1593

data_9013359
_publ_section_title
;Powder neutron-diffraction studies of clinopyroxenes. I. The crystal
 structure and thermoelastic properties of jadeite between 1.5 and 270 K
 Locality: Hweka and Mamon mining district, Burma Note: T = 64.0 K
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1593
_journal_page_last               1622
_journal_paper_doi               10.3749/canmin.46.6.1593
_journal_volume                  46
_journal_year                    2008
_chemical_formula_structural     NaAl(Si2O6)
_chemical_formula_sum            'Al Na O6 Si2'
_chemical_name_mineral           Jadeite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.5662
_cell_angle_gamma                90
_cell_length_a                   9.41599
_cell_length_b                   8.55535
_cell_length_c                   5.22075
_cell_formula_units_Z            4
_cell_volume                     400.957
_diffrn_ambient_temperature      64
_exptl_crystal_density_diffrn    3.349
_cod_original_formula_sum        'Na Al Si2 O6'
_cod_database_code               9013359
Powder neutron-diffraction studies of clinopyroxenes. I. The crystal structure and thermoelastic properties of jadeite between 1.5 and 270 K
Knight, K. S.; Price, G. D.; The Canadian Mineralogist 46 (2008) 1593–1622; doi:10.3749/canmin.46.6.1593

data_9013360
_publ_section_title
;Powder neutron-diffraction studies of clinopyroxenes. I. The crystal
 structure and thermoelastic properties of jadeite between 1.5 and 270 K
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1593
_journal_page_last               1622
_journal_paper_doi               10.3749/canmin.46.6.1593
_journal_volume                  46
_journal_year                    2008
_chemical_compound_source        'Hweka and Mamon mining district, Burma'
_chemical_formula_structural     NaAl(Si2O6)
_chemical_formula_sum            'Al Na O6 Si2'
_chemical_name_mineral           Jadeite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.5670
_cell_angle_gamma                90
_cell_length_a                   9.41607
_cell_length_b                   8.55547
_cell_length_c                   5.22077
_cell_formula_units_Z            4
_cell_volume                     400.966
_database_code_amcsd             0006251
_diffrn_ambient_temperature      73.4
_exptl_crystal_density_diffrn    3.349
_cod_original_formula_sum        'Na Al Si2 O6'
_cod_database_code               9013360